Abstract
We examine the doping effects in the twodimensional periodic Anderson model using the determinant Quantum Monte Carlo (DQMC) method. We observe bound states around the Kondo hole site and find that the heavy electron states are destroyed at the nearestneighbor sites. Our results show no clear sign of hybridization oscillation predicted in previous meanfield calculations. We further study the electron transport with increasing doping and as a function of temperature and obtain a critical doping x_{c} ≈ 0.6 that marks a transition from the Kondo insulator regime to the singleion Kondo regime. The value of x_{c} is in good agreement with the predicted threshold for the site percolation. Our results confirm the percolative nature of the insulatormetal transition widely observed in doped Kondo insulators.
Introduction
Chemical substitution or doping of the magnetic ions (Ce, Yb, U, …) by its nonmagnetic counterpart element (La, Th, Y, …) gives rise to local vacancies of the magnetic fmoments (called the Kondo holes) and could cause dramatic changes in the ground state properties of heavy fermion compounds. In Kondo insulators such as CeNiSn^{1,2,3}, CeRhSb^{2,3}, and Ce_{3}Bi_{4}Pt_{3}^{4}, interesting new physics has been proposed such as the bound states near the Kondo holes^{5,6,7,8,9}. With increasing concentrations of doping, an insulatortometal transition has been widely observed, accompanying with the change from the dense Kondo lattice regime to the singleion Kondo regime. This transition has been generally speculated to be of percolative nature^{10}. Many work, mostly based on meanfield calculations, have been carried out in order to clarify the relevant physics^{7,11}. To the best of our knowledge, no exact numerical calculations has been done. In particular, it is not clear how Kondo holes may destroy the manybody heavy electron state and, with increasing doping, drive the system from the Kondo lattice physics to the singleion Kondo physics.
In this work, we use the determinant Quantum Monte Carlo (DQMC) method to study the electronic and transport properties of the doped twodimensional periodic Anderson lattice. DQMC is an exact numerical method for a finite lattice but often suffers from severe sign problem away from the half filling. We therefore focus on the vicinity of the half filing case and study the doping effect in a Kondo insulator simply by tuning the energy levels of a selected number of local felectron sites. For sufficiently depleted (or doubly occupied) local flevels, this is equivalent to replace the local magnetic ions by the nonmagnetic conterparts. We find no severe sign problem in the considered temperature and tuning range. This allows us to study the evolution of the electronic states with arbitrary number of Kondo holes. We are able to reproduce the predicted bound states around the Kondo hole site obtained in previous meanfield calculations and find that the hybridized heavy electron states are destroyed in the neareastneighbor sites. We further study the electronic transport with increasing doping and confirm the percolation transition from the Kondo insulator state in the dense Kondo lattice to the singleion Kondo behavior in the diluted limit.
Results
We start with the following modified Hamiltonian for the periodic Anderson lattice,
where () and c_{iσ} (f_{iσ}) are the creation and annihilation operators for the conduction and felectrons, respectively. and are the corresponding number operators for the spinσ component on the ith site, t is the hopping parameter of the conduction electrons between the nearestneighbor sites, V describes the local hybridization between the conduction and felectrons, and U is the local Coulomb interaction on the local fsite. represents the felectron energy at the impurity sites I, which is tuned away from zero to resemble the effect of chemical substitution. The sum ∑′ in the last term is only over the impurity sites. We have modified the DQMC code implemented in QUantum Electron Simulation Toolbox^{12} for the tuning and carried out numerical simulations on a 12 × 12 square lattice with a discretization of the imaginary time, Δτ = 0.25. For , the model reduces to a clean Kondo lattice, which has no sign problem due to the particlehole symmetry. For large , the local felectron occupation is effectively empty or full, so the felectron degree of freedom at the impurity site plays essentially no role in the simulation and we also find no severe sign problem. The magnetic and electronic properties of the the felectrons can be obtained through the equaltime spin correlation function^{13,14},
and the imaginary time Green’s function,
The local density of states of the felectrons, ρ_{f;iσ}(ω), can be obtained from G_{f;iσ}(τ) using the maximum entropy method,
The same can be done for the conduction electrons. For simplicity, we set t = 1 and U/t = 6 in the numerical calculations and use the natural units with the Boltzmann constant k_{B} = 1. The large value of U is chosen for typical Kondo lattice systems^{15,16}.
To provide a basis for comparison, we first present the results for the clean lattice () in Fig. 1(e,f). The spin correlation function at low temperature (T/t = 0.05) exhibits clear antiferromagnetic spatial oscillation for V/t = 1.0, indicating antiferromagnetic longrange order in the finite lattice for weak hybridization. For stronger hybridization with V/t = 1.5 and 2.5, the antiferromagnetic oscillation is suppressed and, as expected, the system shows a transition from the antiferromagnetically longrange ordered state to the paramagnetic (disordered) state with increasing hybridization due to the competition between the collective Kondo hybridization and the induced RKKY (RudermanKittelKasuyaYosida) exchange coupling among the fmoments^{17}. Figure 1(f) plots the felectron local density of states at V/t = 1.0. We see for T/t = 0.5 two broad Hubbard peaks located at ω = ±U/2 = ±3. As temperature decreases, a narrow resonance peak first appears at T/t = 0.125, reflecting the onset of coherence, and then splits into two sharp peaks at T/t = 0.05. The split of the resonance peak is a special feature of the Anderson lattice model and originates from the collective hybridization between the conduction band and the effective felectron flat band near the Fermi energy. The emergence of the gap feature indicates that collective hybridization already takes place in the antiferromagnetic state.
The effect of doping can be readily obtained by comparing the results for the clean Anderson lattice () and that with a finite . Figure 1(a–d) plot the spatial distribution of the average , the occupation number of the conduction electrons, for . This resembles the situation of a Kondo hole, as the local felectron occupation number at the impurity site is almost zero. On the other hand, the local occupation of the conduction electrons, , is strongly enhanced and increases rapidly with increasing V. This may be understood if we integrate out the local felectron degree of freedom at the impurity site. We obtain effectively a local attractive potential, , which tends to trap the conduction electrons on the Kondo hole site, causing the increase of . For small V/t = 1.0 and 1.5, we see that is enhanced at the impurity site while slightly reduced in the nearestneighbor sites. The charge density oscillation is also associated with this potential scattering, reflecting the effect of Friedel oscillation of free conduction electrons. This is possible because for sufficiently small V, the scattering potential is relatively stronger and overcomes the hybridization energy, , where a is a constant of the order of unity. As expected, there is no oscillation for strong hybridization at V/t = 2.5. exhibits a rapid decay with increasing distance away from the Kondo hole. We note that unlike previous meanfield studies^{18,19,20}, we observe no evident spatial oscillation in the hybridization function^{21}, indicating that the perturbation is suppressed in our model, possibly due to the half filling.
The perturbation to the local electronic densities of states is presented in Fig. 2 and compared with that far away from the Kondo hole site (FAFH) for V/t = 1.0 and 2.5. The latter is the same as that in the clean lattice. As shown in Fig. 2(a,c), a sharp peak emerges inside the hybridization gap for both ρ_{c} at the Kondo hole site and ρ_{f} at the nearestneighbor sites for V/t = 2.5, in contrast to the unperturbed results far away from the Kondo hole site. The resonance peak gives the wellknown bound states and is missing if hybridization strength at the hole site is set to zero (no impurity scattering). For small V, the bound states are absent due to weak impurity scattering as discussed above and the peaks at the edges of the hybridization gap reflect the hybridization between the conduction electrons and the fmoments, similar to those in the clean lattice. The suppression of these hybridization states at the gap edges for V/t = 2.5 is a manifestation of the destruction of the heavy electrons due to the presence of the nearby Kondo hole. This suggests that the heavy electron emergence is not a singlesite property but a collective phenomenon that involves correlations among neighboring sites in the dense Kondo lattice.
Figure 3 further compares the densities of states at different sites and for varying . We see that the height of the resonance peak is reduced substantially by over an order of magnitude further away from the impurity site. Nevertheless, as increases, the bound states move uniformly towards the center of the hybridization gap and become more and more pronounced. The change in their location is shown as a function of in the inset of Fig. 3(c). We obtain similar curves for the peaks in both ρ_{c} at the hole site and ρ_{f} at the NN sites, indicating their common origin. As expected, the bound state approaches ω = 0 as , consistent with the meanfield prediction.
Next, we study how increasing doping may change the electronic and transport properties by tuning the system from the Kondo insulator to the diluted limit. We add more impurity sites whose positions are chosen randomly in the numerical simulation and calculate the dc conductivity of the doped Anderson lattice using the approximation,
in which g_{xx}(τ) is the currentcurrent correlation function in imaginary time,
with
The resulting conductivity, σ_{dc}, is plotted in Fig. 4 as a function of doping x for different temperatures. The data presented here are an average over only 5 samples of random configurations. We have checked the results up to 20 samples and found a numerical error of less than 5%. We see all curves cross at a critical doping, x_{c} ≈ 0.6, indicating opposite temperature dependence below and above x_{c}. Moreover, our analysis of finite size effect shows no significant change in x_{c} with increasing L (see Supplementary Fig. S1). For x < 0.6, σ_{dc} is small and the resistivity, ρ = 1/σ_{dc}, increases as temperature decreases, so that the system is in the Kondo insulator phase. As x becomes larger than 0.6, σ_{dc} increases rapidly with x as the system approaches the singleion Kondo limit. In this regime, ρ(T) first decreases with deceasing temperature and exhibits metallic behavior at high temperatures down to about T < 0.1, below which the resistivity becomes insulating like, with a minimum signalling the typical singleion Kondo behavior in the diluted limit. Our calculations therefore cover the whole doping range from the dense Kondo lattice to the singleion Kondo limit.
To understand the connection between the transport property and the bound states, we calculate the average densities of states of both the conduction and felectrons on all sites. The results are plotted in Fig. 4(c,d). We see that the average impurity states exhibit broad peaks inside the hybridization gap, similar to the meanfield results. For x = 0.333, 0.583 and 0.667, the gap is gradually filled in, yielding a finite density of states at ω = 0, in contrast to the insulating like behavior shown in our calculated resistivity curve. Hence the average density of states cannot be used directly to explain the transport properties. This points to the percolative nature of the electron transport. In the theory of site percolation^{10}, adjacent bound states could form a cluster. When the size of the cluster grows and eventually percolates through the whole lattice after stochastic doping of enough sites, the system reaches a percolation threshold where a phase transition takes place. For the square lattice of infinite size in two dimension with only nearestneighbor hopping, the percolation threshold is x_{c} ≈ 0.593^{10}. Increasing the number of coordination or dimension can reduce the threshold^{9}. In our two dimensional 12 × 12 system, bound states are only pronounced at the hole site for the conduction electrons. Since only nearestneighbor hopping is allowed, the impurity sites have to be connected to form a network in order for the conduction electrons to move from one side to the other side of the lattice. As shown in Fig. 4, the critical doping x_{c} ≈ 0.6 obtained in our resistivity calculations is in good agreement with the percolation threshold x_{c}. Moreover, previous theories have also predicted for T = 0 and x > x_{c} a power law scaling, σ_{dc} ∝ (x − x_{c})^{μ}, with μ ≈ 1.3^{22}, consistent with our fit giving μ ≈ 1.44 for L = 12 and βt = 16 (see Supplementary Fig. S2). The dopinginduced insulatormetal transition is therefore an indication of site percolation of the conducting electrons through the bound states, which governs the charge transport in the heavily doped Kondo lattice. Our results confirm the previous theoretical and experimental speculations. Along the percolation path, collective hybridizations are destroyed around the impurity sites, providing an explanation to the crossover from the heavy electron physics to the singleion Kondo physics.
Conclusion
We use the determinant Quantum Monte Carlo (DQMC) method to study the doping effects in the twodimensional periodic Anderson lattice. We observe the suppression of the hybridization feature in the vicinity of the Kondo hole, which suggests a physical mechanism to destroy the heavy electron states with increasing doping. Our results also confirm the bound states appearing around the Kondo hole, but show no obvious signature of the hybridization oscillation predicted in the meanfield calculations. We further study the evolution of the electron transport with increasing doping and demonstrate the percolative nature of the insulatormetal transition from the dense Kondo lattice to the singleion Kondo limit. We obtain a critical doping that is consistent with the predicted threshold for site percolation.
Additional Information
How to cite this article: Wei, L. and Yang, Y. Dopinginduced perturbation and percolation in the twodimensional Anderson lattice. Sci. Rep. 7, 46089; doi: 10.1038/srep46089 (2017).
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
References
Echizen, Y. & Takabatake, T. Effect of Kondohole impurity on the pseudogap in CeNiSn. Physica B: Conden. Mat. 259, 292–293 (1999).
Adroja, D. T., Rainford, B. D., Neville, A. J., Mandal, P. & Jansen, A. G. M. A comparative study of suppression of the energy gap with La substitution in the Kondo insulators: CeNiSn and CeRhSb. J. Magn. Magn. Mater. 161, 157–168 (1996).
Goraus, J. & Ślebarski, A. Quantum critical transition from Kondo insulator to metallic state studied by bandstructure calculations for doped compounds: CeRhSb and CeNiSn. Phys. Status Solidi B 250, 533–536 (2013).
Pietrus, T. & Löhneysen, H. v. & Schlottmann, P. Kondohole conduction in the Ladoped Kondo insulator Ce3Bi4Pt3 . Phys. Rev. B 77, 115134 (2008).
Sollie, R. & Schlottmann, P. A simple theory of the Kondo hole. J. Appl. Phys. 69, 5478–5480 (1991).
Sollie, R. & Schlottmann, P. Local density of states in the vicinity of a Kondo hole. J. Appl. Phys. 70, 5803–5805 (1991).
Schlottmann, P. Impurity bands in Kondo insulators. Phys. Rev. B 46, 998–1004 (1992).
Schlottmann, P. Influence of a Kondohole impurity band on magnetic instabilities in Kondo insulators. Phys. Rev. B 54, 12324–12331 (1996).
Schlottmann, P. & Hellberg, C. S. Metalinsulator transition in dirty Kondo insulators. J. Appl. Phys. 79, 6414–6416 (1996).
Aharony, A. & Stauffer, D. Introduction to percolation theory (Taylor & Francis, 2003).
Li, Z.z., Xu, W., Chen, C. & Xiao, M.w. Alloying effects of Kondo insulators. Phys. Rev. B 50, 11332–11339 (1994).
Tomas, A., Chang, C.C., Scalettar, R. & Bai, Z. Advancing large scale manybody QMC simulations on GPU accelerated multicore systems. In Parallel & Distributed Processing Symposium (IPDPS), 2012 IEEE 26th International 308–319 (IEEE, 2012).
Hirsch, J. E. & Tang, S. Antiferromagnetism in the twodimensional Hubbard model. Phys. Rev. Lett. 62, 591–594 (1989).
Vekić, M., Cannon, J. W., Scalapino, D. J., Scalettar, R. T. & Sugar, R. L. Competition between antiferromagnetic order and spinliquid behavior in the twodimensional periodic Anderson model at half filling. Phys. Rev. Lett. 74, 2367–2370 (1995).
Jiang, M., Curro, N. J. & Scalettar, R. T. Universal knight shift anomaly in the periodic anderson model. Phys. Rev. B 90, 241109 (2014).
Shim, J., Haule, K. & Kotliar, G. Modeling the localizedtoitinerant electronic transition in the heavy fermion system CeIrIn5 . Science 318, 1615–1617 (2007).
Doniach, S. The Kondo lattice and weak antiferromagnetism. Physica B + C 91, 231–234 (1977).
Figgins, J. & Morr, D. K. Defects in heavyfermion materials: unveiling strong correlations in real space. Phys. Rev. Lett. 107, 066401 (2011).
Toldin, F. P., Figgins, J., Kirchner, S. & Morr, D. K. Disorder and quasiparticle interference in heavyfermion materials. Phys. Rev. B 88, 081101 (2013).
Zhu, J.X., Julien, J.P., Dubi, Y. & Balatsky, A. V. Local electronic structure and fano interference in tunneling into a Kondo hole system. Phys. Rev. Lett. 108, 186401 (2012).
Hamidian, M. H. et al. How Kondoholes create intense nanoscale heavyfermion hybridization disorder. Proc. Natl. Acad. Sci. USA 108, 18233–18237 (2011).
Clerc, J., Giraud, G., Laugier, J. & Luck, J. The electrical conductivity of binary disordered systems, percolation clusters, fractals and related models. Adv. Phys. 39, 191–309 (1990).
Acknowledgements
This work was supported by the National Natural Science Foundation of China (NSFC Grant No. 11522435), the State Key Development Program for Basic Research of China (Grant No. 2015CB921303), the Strategic Priority Research Program (B) of the Chinese Academy of Sciences (Grant No. XDB07020200) and the Youth Innovation Promotion Association CAS.
Author information
Authors and Affiliations
Contributions
Y.Y. conceived the idea. Y.Y. and L.W. performed the research and wrote the paper.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Wei, Ly., Yang, Yf. Dopinginduced perturbation and percolation in the twodimensional Anderson lattice. Sci Rep 7, 46089 (2017). https://doi.org/10.1038/srep46089
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/srep46089
This article is cited by

Hybridization oscillation in the onedimensional KondoHeisenberg model with Kondo holes
Scientific Reports (2017)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.